Natural rubber - wikipedia Natural rubber `` Rubber '' and `` India rubber '' redirect here. For other uses, see Rubber ( disambiguation ). This article is about the polymeric material `` natural rubber ''. For man - made rubber materials, see Synthetic rubber. This article needs additional citations for verification. Please help improve this article by adding citations to reliable sources. Unsourced material may be challenged and removed. ( September 2016 ) Latex being collected from a tapped rubber tree, Cameroon Rubber tree plantation in Thailand Natural rubber, also called India rubber or caoutchouc, as initially produced, consists of polymers of the organic compound isoprene, with minor impurities of other organic compounds, plus water. Malaysia and Indonesia are two of the leading rubber producers. Forms of polyisoprene that are used as natural rubbers are classified as elastomers. Currently, rubber is harvested mainly in the form of the latex from the rubber tree or others. The latex is a sticky, milky colloid drawn off by making incisions in the bark and collecting the fluid in vessels in a process called `` tapping ''. The latex then is refined into rubber ready for commercial processing. In major areas, latex is allowed to coagulate in the collection cup. The coagulated lumps are collected and processed into dry forms for marketing. Natural rubber is used extensively in many applications and products, either alone or in combination with other materials. In most of its useful forms, it has a large stretch ratio and high resilience, and is extremely waterproof. Contents 1 Varieties 1.1 Hevea brasiliensis 1.2 Congo rubber 1.3 Dandelion 1.4 Other 2 History 2.1 Pre-World War II 3 Properties 3.1 Elasticity 4 Chemical makeup 4.1 Biosynthesis 5 Production 5.1 Cultivation 5.2 Collection 5.2. 1 Field coagula 5.2. 1.1 Cup lump 5.2. 1.2 Tree lace 5.2. 1.3 Smallholders ' lump 5.2. 1.4 Earth scrap 5.3 Processing 5.4 Vulcanized rubber 5.5 Transportation 6 Uses 7 Allergic reactions 8 Microbial degradation 9 See also 10 References 10.1 Notes 10.2 Bibliography 11 External links Varieties Hevea brasiliensis The major commercial source of natural rubber latex is the Pará rubber tree ( Hevea brasiliensis ), a member of the spurge family, Euphorbiaceae. This species is preferred because it grows well under cultivation. A properly managed tree responds to wounding by producing more latex for several years. Congo rubber Congo rubber, formerly a major source of rubber, came from vines in the genus Landolphia ( L. kirkii, L. heudelotis, and L. owariensis ). These can not be cultivated, and the intense drive to collect latex from wild plants was responsible for many of the atrocities committed under the Congo Free State. Dandelion Dandelion milk contains latex. The latex exhibits the same quality as the natural rubber from rubber trees. In the wild types of dandelion, latex content is low and varies greatly. In Nazi Germany, research projects tried to use dandelions as a base for rubber production, but failed. In 2013, by inhibiting one key enzyme and using modern cultivation methods and optimization techniques, scientists in the Fraunhofer Institute for Molecular Biology and Applied Ecology ( IME ) in Germany developed a cultivar that is suitable for commercial production of natural rubber. In collaboration with Continental Tires, IME began a pilot facility. Other Many other plants produce forms of latex rich in isoprene polymers, though not all produce usable forms of polymer as easily as the Pará. Some of them require more elaborate processing to produce anything like usable rubber, and most are more difficult to tap. Some produce other desirable materials, for example gutta - percha ( Palaquium gutta ) and chicle from Manilkara species. Others that have been commercially exploited, or at least showed promise as rubber sources, include the rubber fig ( Ficus elastica ), Panama rubber tree ( Castilla elastica ), various spurges ( Euphorbia spp. ), lettuce ( Lactuca species ), the related Scorzonera tau - saghyz, various Taraxacum species, including common dandelion ( Taraxacum officinale ) and Russian dandelion ( Taraxacum kok - saghyz ), and perhaps most importantly for its hypoallergenic properties, guayule ( Parthenium argentatum ). The term gum rubber is sometimes applied to the tree - obtained version of natural rubber in order to distinguish it from the synthetic version. History The first use of rubber was by the indigenous cultures of Mesoamerica. The earliest archeological evidence of the use of natural latex from the Hevea tree comes the Olmec culture, in which rubber was first used for making balls for the Mesoamerican ballgame. Rubber was later used by the Maya and Aztec cultures - in addition to making balls Aztecs used rubber for other purposes such as making containers and to make textiles waterproof by impregnating them with the latex sap. The Pará rubber tree is indigenous to South America. Charles Marie de La Condamine is credited with introducing samples of rubber to the Académie Royale des Sciences of France in 1736. In 1751, he presented a paper by François Fresneau to the Académie ( published in 1755 ) that described many of rubber 's properties. This has been referred to as the first scientific paper on rubber. In England, Joseph Priestley, in 1770, observed that a piece of the material was extremely good for rubbing off pencil marks on paper, hence the name `` rubber ''. It slowly made its way around England. In 1764 François Fresnau discovered that turpentine was a rubber solvent. Giovanni Fabbroni is credited with the discovery of naphtha as a rubber solvent in 1779. South America remained the main source of the limited amounts of latex rubber used during much of the 19th century. The trade was heavily protected and exporting seeds from Brazil was a capital offense, although no law prohibited it. Nevertheless, in 1876, Henry Wickham smuggled 70,000 Pará rubber tree seeds from Brazil and delivered them to Kew Gardens, England. Only 2,400 of these germinated. Seedlings were then sent to India, British Ceylon ( Sri Lanka ), Dutch East Indies ( Indonesia ), Singapore, and British Malaya. Malaya ( now Peninsular Malaysia ) was later to become the biggest producer of rubber. In the early 1900s, the Congo Free State in Africa was also a significant source of natural rubber latex, mostly gathered by forced labor. Liberia and Nigeria started production. In India, commercial cultivation was introduced by British planters, although the experimental efforts to grow rubber on a commercial scale were initiated as early as 1873 at the Calcutta Botanical Gardens. The first commercial Hevea plantations were established at Thattekadu in Kerala in 1902. In later years the plantation expanded to Karnataka, Tamil Nadu and the Andaman and Nicobar Islands of India. India today is the world 's 3rd largest producer and 4th largest consumer. In Singapore and Malaya, commercial production was heavily promoted by Sir Henry Nicholas Ridley, who served as the first Scientific Director of the Singapore Botanic Gardens from 1888 to 1911. He distributed rubber seeds to many planters and developed the first technique for tapping trees for latex without causing serious harm to the tree. Because of his fervent promotion of this crop, he is popularly remembered by the nickname `` Mad Ridley ''. Pre-world War II Charles Goodyear developed vulcanization in 1839, although Mesoamericans used stabilized rubber for balls and other objects as early as 1600 BC. Before World War II significant uses included door and window profiles, hoses, belts, gaskets, matting, flooring and dampeners ( antivibration mounts ) for the automotive industry. The use of rubber in car tires ( initially solid rather than pneumatic ) in particular consumed a significant amount of rubber. Gloves ( medical, household and industrial ) and toy balloons were large consumers of rubber, although the type of rubber used is concentrated latex. Significant tonnage of rubber was used as adhesives in many manufacturing industries and products, although the two most noticeable were the paper and the carpet industries. Rubber was commonly used to make rubber bands and pencil erasers. Rubber produced as a fiber, sometimes called ' elastic ', had significant value to the textile industry because of its excellent elongation and recovery properties. For these purposes, manufactured rubber fiber was made as either an extruded round fiber or rectangular fibers cut into strips from extruded film. Because of its low dye acceptance, feel and appearance, the rubber fiber was either covered by yarn of another fiber or directly woven with other yarns into the fabric. Rubber yarns were used in foundation garments. While rubber is still used in textile manufacturing, its low tenacity limits its use in lightweight garments because latex lacks resistance to oxidizing agents and is damaged by aging, sunlight, oil and perspiration. The textile industry turned to neoprene ( polymer of chloroprene ), a type of synthetic rubber, as well as another more commonly used elastomer fiber, spandex ( also known as elastane ), because of their superiority to rubber in both strength and durability. Properties Rubber latex Rubber exhibits unique physical and chemical properties. Rubber 's stress -- strain behavior exhibits the Mullins effect and the Payne effect and is often modeled as hyperelastic. Rubber strain crystallizes. Due to the presence of a double bond in each repeat unit, natural rubber is susceptible to vulcanisation and sensitive to ozone cracking. The two main solvents for rubber are turpentine and naphtha ( petroleum ). Because rubber does not dissolve easily, the material is finely divided by shredding prior to its immersion. An ammonia solution can be used to prevent the coagulation of raw latex. Rubber begins to melt at approximately 180 ° C ( 356 ° F ). Natural rubber has a strong, unpleasant odour. Elasticity Main article : Rubber elasticity This section needs additional citations for verification. Please help improve this article by adding citations to reliable sources. Unsourced material may be challenged and removed. ( August 2015 ) On a microscopic scale, relaxed rubber is a disorganized cluster of erratically changing wrinkled chains. In stretched rubber, the chains are almost linear. The restoring force is due to the preponderance of wrinkled conformations over more linear ones. For the quantitative treatment see ideal chain, for more examples see entropic force. Cooling below the glass transition temperature permits local conformational changes but a reordering is practically impossible because of the larger energy barrier for the concerted movement of longer chains. `` Frozen '' rubber 's elasticity is low and strain results from small changes of bond lengths and angles : this caused the Challenger disaster, when the American Space Shuttle 's flattened o - rings failed to relax to fill a widening gap. The glass transition is fast and reversible : the force resumes on heating. The parallel chains of stretched rubber are susceptible to crystallization. This takes some time because turns of twisted chains have to move out of the way of the growing crystallites. Crystallization has occurred, for example, when, after days, an inflated toy balloon is found withered at a relatively large remaining volume. Where it is touched, it shrinks because the temperature of the hand is enough to melt the crystals. Vulcanization of rubber creates disulfide bonds between chains, which limits the degrees of freedom and results in chains that tighten more quickly for a given strain, thereby increasing the elastic force constant and making the rubber harder and less extensible. Chemical makeup Chemical structure of cis - polyisoprene, the main constituent of natural rubber. Synthetic cis - polyisoprene and natural cis - polyisoprene are derived from different precursors, isopentenyl pyrophosphate and isoprene. Latex is the polymer cis - 1, 4 - polyisoprene -- with a molecular weight of 100,000 to 1,000,000 daltons. Typically, a small percentage ( up to 5 % of dry mass ) of other materials, such as proteins, fatty acids, resins, and inorganic materials ( salts ) are found in natural rubber. Polyisoprene can also be created synthetically, producing what is sometimes referred to as `` synthetic natural rubber '', but the synthetic and natural routes are different. Some natural rubber sources, such as gutta - percha, are composed of trans - 1, 4 - polyisoprene, a structural isomer that has similar properties. Natural rubber is an elastomer and a thermoplastic. Once the rubber is vulcanized, it turns into a thermoset. Most rubber in everyday use is vulcanized to a point where it shares properties of both ; i.e., if it is heated and cooled, it is degraded but not destroyed. The final properties of a rubber item depend not just on the polymer, but also on modifiers and fillers, such as carbon black, factice, whiting and others. Biosynthesis Rubber particles are formed in the cytoplasm of specialized latex - producing cells called laticifers within rubber plants. Rubber particles are surrounded by a single phospholipid membrane with hydrophobic tails pointed inward. The membrane allows biosynthetic proteins to be sequestered at the surface of the growing rubber particle, which allows new monomeric units to be added from outside the biomembrane, but within the lacticifer. The rubber particle is an enzymatically active entity that contains three layers of material, the rubber particle, a biomembrane and free monomeric units. The biomembrane is held tightly to the rubber core due to the high negative charge along the double bonds of the rubber polymer backbone. Free monomeric units and conjugated proteins make up the outer layer. The rubber precursor is isopentenyl pyrophosphate ( an allylic compound ), which elongates by Mg - dependent condensation by the action of rubber transferase. The monomer adds to the pyrophosphate end of the growing polymer. The process displaces the terminal high - energy pyrophosphate. The reaction produces a cis polymer. The initiation step is catalyzed by prenyltransferase, which converts three monomers of isopentenyl pyrophosphate into farnesyl pyrophosphate. The farnesyl pyrophosphate can bind to rubber transferase to elongate a new rubber polymer. The required isopentenyl pyrophosphate is obtained from the mevalonate pathway, which derives from acetyl - CoA in the cytosol. In plants, isoprene pyrophosphate can also be obtained from the 1 - deox - D - xyulose - 5 - phosphate / 2 - C - methyl - D - erythritol - 4 - phosphate pathway within plasmids. The relative ratio of the farnesyl pyrophosphate initiator unit and isoprenyl pyrophosphate elongation monomer determines the rate of new particle synthesis versus elongation of existing particles. Though rubber is known to be produced by only one enzyme, extracts of latex host numerous small molecular weight proteins with unknown function. The proteins possibly serve as cofactors, as the synthetic rate decreases with complete removal. Production Rubber is generally cultivated in large plantations. The image shows a coconut shell used in collecting latex, in plantations in Kerala, India. Close to 28 million tons of rubber were produced in 2013, of which approximately 44 % was natural. Since the bulk is synthetic, which is derived from petroleum, the price of natural rubber is determined, to a large extent, by the prevailing global price of crude oil. Asia was the main source of natural rubber, accounting for about 94 % of output in 2005. The three largest producers, Thailand, Indonesia ( 2.4 million tons ) and Malaysia, together account for around 72 % of all natural rubber production. Natural rubber is not cultivated widely in its native continent of South America due to the existence of South American leaf blight, and other natural predators. Cultivation Rubber latex is extracted from rubber trees. The economic life period of rubber trees in plantations is around 32 years -- up to 7 years of immature phase and about 25 years of productive phase. The soil requirement is well - drained, weathered soil consisting of laterite, lateritic types, sedimentary types, nonlateritic red or alluvial soils. The climatic conditions for optimum growth of rubber trees are : Rainfall of around 250 centimetres ( 98 in ) evenly distributed without any marked dry season and with at least 100 rainy days per year Temperature range of about 20 to 34 ° C, with a monthly mean of 25 to 28 ° C Atmospheric humidity of around 80 % About 2000 hours sunshine per year at the rate of six hours per day throughout the year Absence of strong winds Many high - yielding clones have been developed for commercial planting. These clones yield more than 2,000 kg of dry rubber per hectare per year, under ideal conditions. Collection A woman in Sri Lanka harvesting rubber, circa 1920 In places such as Kerala where coconuts are in abundance, the half shell of coconut was used as the latex collection container. Glazed pottery or aluminium or plastic cups became more common in Kerala and other countries. The cups are supported by a wire that encircles the tree. This wire incorporates a spring so it can stretch as the tree grows. The latex is led into the cup by a galvanised `` spout '' knocked into the bark. Tapping normally takes place early in the morning, when the internal pressure of the tree is highest. A good tapper can tap a tree every 20 seconds on a standard half - spiral system, and a common daily `` task '' size is between 450 and 650 trees. Trees are usually tapped on alternate or third days, although many variations in timing, length and number of cuts are used. The latex, which contains 30 -- 40 % dry rubber, is in the bark, so the tapper must avoid cutting right through to the wood, else the growing cambial layer is damaged and the renewing bark becomes deformed, making later tapping difficult. It is usual to tap a pannel at least twice, sometimes three times, during the tree 's life. The economic life of the tree depends on how well the tapping is carried out, as the critical factor is bark consumption. A standard in Malaysia for alternate daily tapping is 25 cm ( vertical ) bark consumption per year. The latex - containing tubes in the bark ascend in a spiral to the right. For this reason, tapping cuts usually ascend to the left to cut more tubes. The trees drip latex for about four hours, stopping as latex coagulates naturally on the tapping cut, thus blocking the latex tubes in the bark. Tappers usually rest and have a meal after finishing their tapping work, then start collecting the liquid `` field latex '' at about midday. Field coagula Mixed field coagula. Smallholder 's lump at a remilling factory The four types of field coagula are `` cuplump '', `` treelace '', `` smallholders ' lump '' and `` earth scrap ''. Each has significantly different properties. Some trees continue to drip after the collection leading to a small amount of `` cup lump '' that is collected at the next tapping. The latex that coagulates on the cut is also collected as `` tree lace ''. Tree lace and cup lump together account for 10 -- 20 % of the dry rubber produced. Latex that drips onto the ground, `` earth scrap '', is also collected periodically for processing of low - grade product. Cup lump Cup lump is the coagulated material found in the collection cup when the tapper next visits the tree to tap it again. It arises from latex clinging to the walls of the cup after the latex was last poured into the bucket, and from late - dripping latex exuded before the latex - carrying vessels of the tree become blocked. It is of higher purity and of greater value than the other three types. Tree lace Tree lace is the coagulum strip that the tapper peels off the previous cut before making a new cut. It usually has higher copper and manganese contents than cup lump. Both copper and manganese are pro-oxidants and can damage the physical properties of the dry rubber. Smallholders ' lump Smallholders ' lump is produced by smallholders who collect rubber from trees far from the nearest factory. Many Indonesian smallholders, who farm paddies in remote areas, tap dispersed trees on their way to work in the paddy fields and collect the latex ( or the coagulated latex ) on their way home. As it is often impossible to preserve the latex sufficiently to get it to a factory that processes latex in time for it to be used to make high quality products, and as the latex would anyway have coagulated by the time it reached the factory, the smallholder will coagulate it by any means available, in any container available. Some smallholders use small containers, buckets etc., but often the latex is coagulated in holes in the ground, which are usually lined with plastic sheeting. Acidic materials and fermented fruit juices are used to coagulate the latex -- a form of assisted biological coagulation. Little care is taken to exclude twigs, leaves, and even bark from the lumps that are formed, which may also include tree lace. Earth scrap Earth scrap is material that gathers around the base of the tree. It arises from latex overflowing from the cut and running down the bark, from rain flooding a collection cup containing latex, and from spillage from tappers ' buckets during collection. It contains soil and other contaminants, and has variable rubber content, depending on the amount of contaminants. Earth scrap is collected by field workers two or three times a year and may be cleaned in a scrap - washer to recover the rubber, or sold off to a contractor who cleans it and recovers the rubber. It is of low quality. Processing Removing coagulum from coagulating troughs. Latex coagulates in the cups if kept for long and must be collected before this happens. The collected latex, `` field latex '', is transferred into coagulation tanks for the preparation of dry rubber or transferred into air - tight containers with sieving for ammoniation. Ammoniation preserves the latex in a colloidal state for longer periods of time. Latex is generally processed into either latex concentrate for manufacture of dipped goods or coagulated under controlled, clean conditions using formic acid. The coagulated latex can then be processed into the higher - grade, technically specified block rubbers such as SVR 3L or SVR CV or used to produce Ribbed Smoke Sheet grades. Naturally coagulated rubber ( cup lump ) is used in the manufacture of TSR10 and TSR20 grade rubbers. Processing for these grades is a size reduction and cleaning process to remove contamination and prepare the material for the final stage of drying. The dried material is then baled and palletized for storage and shipment. Vulcanized rubber Main article : Vulcanization Torn latex rubber dry suit wrist seal Natural rubber is often vulcanized, a process by which the rubber is heated and sulfur, peroxide or bisphenol are added to improve resistance and elasticity and to prevent it from perishing. Before World War II, carbon black was often used as an additive to rubber to improve its strength, especially in vehicle tires. Transportation Natural rubber latex is shipped from factories in south - west Asia, South America, and West and Center Africa to destinations around the world. As the cost of natural rubber has risen significantly and rubber products are dense, the shipping methods offer the lowest cost per unit weight are preferred. Depending on destination, warehouse availability, and transportation conditions, some methods are preferred by certain buyers. In international trade, latex rubber is mostly shipped in 20 - foot ocean containers. Inside the container, smaller containers are used to store the latex. Uses Compression molded ( cured ) rubber boots before the flashes are removed This section needs additional citations for verification. Please help improve this article by adding citations to reliable sources. Unsourced material may be challenged and removed. ( November 2016 ) This section possibly contains original research. Please improve it by verifying the claims made and adding inline citations. Statements consisting only of original research should be removed. ( November 2016 ) Uncured rubber is used for cements ; for adhesive, insulating, and friction tapes ; and for crepe rubber used in insulating blankets and footwear. Vulcanized rubber has many more applications. Resistance to abrasion makes softer kinds of rubber valuable for the treads of vehicle tires and conveyor belts, and makes hard rubber valuable for pump housings and piping used in the handling of abrasive sludge. The flexibility of rubber is appealing in hoses, tires and rollers for devices ranging from domestic clothes wringers to printing presses ; its elasticity makes it suitable for various kinds of shock absorbers and for specialized machinery mountings designed to reduce vibration. Its relative gas impermeability makes it useful in the manufacture of articles such as air hoses, balloons, balls and cushions. The resistance of rubber to water and to the action of most fluid chemicals has led to its use in rainwear, diving gear, and chemical and medicinal tubing, and as a lining for storage tanks, processing equipment and railroad tank cars. Because of their electrical resistance, soft rubber goods are used as insulation and for protective gloves, shoes and blankets ; hard rubber is used for articles such as telephone housings, parts for radio sets, meters and other electrical instruments. The coefficient of friction of rubber, which is high on dry surfaces and low on wet surfaces, leads to its use for power - transmission belting and for water - lubricated bearings in deep - well pumps. Indian rubber balls or lacrosse balls are made of rubber. Around 25 million tonnes of rubber are produced each year, of which 30 percent is natural. The remainder is synthetic rubber derived from petrochemical sources. The top end of latex production results in latex products such as surgeons ' gloves, condoms, balloons and other relatively high - value products. The mid-range which comes from the technically specified natural rubber materials ends up largely in tires but also in conveyor belts, marine products, windshield wipers and miscellaneous goods. Natural rubber offers good elasticity, while synthetic materials tend to offer better resistance to environmental factors such as oils, temperature, chemicals and ultraviolet light. `` Cured rubber '' is rubber that has been compounded and subjected to the vulcanisation process to create cross-links within the rubber matrix. Allergic reactions Main article : Latex allergy Some people have a serious latex allergy, and exposure to natural latex rubber products such as latex gloves can cause anaphylactic shock. The antigenic proteins found in Hevea latex may be deliberately reduced ( though not eliminated ) through processing. Latex from non-Hevea sources, such as Guayule, can be used without allergic reaction by persons with an allergy to Hevea latex. Some allergic reactions are not to the latex itself, but from residues of chemicals used to accelerate the cross-linking process. Although this may be confused with an allergy to latex, it is distinct from it, typically taking the form of Type IV hypersensitivity in the presence of traces of specific processing chemicals. Microbial degradation Natural rubber is susceptible to degradation by a wide range of bacteria.. The bacteria Streptomyces coelicolor, Pseudomonas citronellolis, and Nocardia spp. are capable of degrading vulcanized natural rubber. See also Akron, Ohio, center of the US rubber industry Condoms, also called `` rubbers '' Crepe rubber Ebonite Emulsion dispersion Fordlândia, failed attempt to establish a rubber plantation in Brazil Reinforced rubber Resilin, a rubber substitute Rubber seed oil Rubber technology Stevenson Plan, historical British plan to stabilize rubber prices Charles Greville Williams, researched natural rubber being a polymer of the monomer isoprene References Notes ^ Jump up to : Heinz - Hermann Greve `` Rubber, 2. Natural '' in Ullmann 's Encyclopedia of Industrial Chemistry, 2000, Wiley - VCH, Weinheim. doi : 10.1002 / 14356007. a23_225 Jump up ^ `` Rubber and Other Latex Products ''. Retrieved 31 August 2014. Jump up ^ Heim, Susanne ( 2002 ). Autarkie und Ostexpansion : Pflanzenzucht und Agrarforschung im Nationalsozialismus. Wallstein Verlag. ISBN 978 - 3 - 89244 - 496 - 1. Jump up ^ `` Making Rubber from Dandelion Juice ''. Science Daily. October 28, 2013. Retrieved 22 November 2013. Jump up ^ Burns, Bill. `` The Gutta Percha Company ''. History of the Atlantic Cable & Undersea Communications. Retrieved 14 February 2009. Jump up ^ Emory Dean Keoke, Kay Marie Porterfield. 2009. Encyclopedia of American Indian Contributions to the World : 15,000 Years of Inventions and Innovations. Infobase Publishing Jump up ^ John Tully. 2011. The Devil 's Milk : A Social History of Rubber. NYU Press ^ Jump up to : `` Charles Marie de la Condamine ''. bouncing-balls.com. Jump up ^ `` Natural rubber in India ''. Jump up ^ Cornelius - Takahama, Vernon ( 2001 ). `` Sir Henry Nicholas Ridley ''. Singapore Infopedia. Archived from the original on 4 May 2013. Retrieved 9 February 2013. Jump up ^ Leng, Dr Loh Wei ; Keong, Khor Jin ( 19 September 2011 ). `` Mad Ridley and the rubber boom ''. Malaysia History. Retrieved 9 February 2013. Jump up ^ Hosler, D. ; Burkett, S.L. ; Tarkanian, M.J. ( 1999 ). `` Prehistoric polymers : Rubber processing in ancient Mesoamerica ''. Science. 284 ( 5422 ) : 1988 -- 1991. PMID 10373117. doi : 10.1126 / science. 284.5422. 1988. Jump up ^ Slack, Charles ( 7 August 2002 ). Noble obsession : Charles Goodyear, Thomas Hancock, and the race to unlock the greatest industrial secret of the nineteenth century. Hyperion. ISBN 978 - 0 - 7868 - 6789 - 9. Jump up ^ `` Casing Joint Design '' ( PDF ). Report - Investigation of the Challenger Accident. US Government Printing Office. Retrieved August 29, 2015. Jump up ^ Koyama, Tanetoshi ; Steinbüchel, Alexander, eds. ( June 2011 ). `` Biosynthesis of Natural Rubber and Other Natural Polyisoprenoids ''. Polyisoprenoids. Biopolymers. 2. Wiley - Blackwell. pp. 73 -- 81. ISBN 978 - 3 - 527 - 30221 - 5. Jump up ^ Paterson - Jones, J.C. ; Gilliland, M.G. ; Van Staden, J. ( June 1990 ). `` The Biosynthesis of Natural Rubber ''. Journal of Plant Physiology. 136 ( 3 ) : 257 -- 263. ISSN 0176 - 1617. doi : 10.1016 / S0176 - 1617 ( 11 ) 80047 - 7. Jump up ^ Schulze Gronover, Christian ; Wahler, Daniela ; Prufer, Dirk ( 5 Jul 2011 ). `` 4. Natural Rubber Biosynthesis and Physic - Chemical Studies on Plant Derived Latex ''. In Magdy, Elnashar. Biotechnology of Biopolymers. ISBN 978 - 953 - 307 - 179 - 4. Jump up ^ Xie, W. ; McMahan, C.M. ; Distefano, A.J. DeGraw, M.D. ; et al. ( 2008 ). `` Initiation of rubber synthesis : In vitro comparisons of benzophenone - modified diphosphate analogues in three rubber preducing species ''. Phytochemistry. 69 : 2539 -- 2545. PMID 18799172. doi : 10.1016 / j. phytochem. 2008.07. 011. Jump up ^ Casey, P.J. ; Seabra, M.C. ( 1996 ). `` Protein Prenyltransferases ''. Journal of Biological Chemistry. 271 ( 10 ) : 5289 -- 5292. PMID 8621375. doi : 10.1074 / jbc. 271.10. 5289. Jump up ^ Kang, H. ; Kang, M.Y. ; Han, K.H. ( 2000 ). `` Identification of Natural Rubber and Characterization of Biosynthetic Activity ''. Plant Physiol. 123 ( 3 ) : 1133 -- 1142. doi : 10.1104 / pp. 123.3. 1133. Jump up ^ `` Overview of the Causes of Natural Rubber Price Volatility ''. En.wlxrubber.com. 1 February 2010. Archived from the original on 26 May 2013. Retrieved 21 March 2013. Jump up ^ `` STATISTICAL SUMMARY OF WORLD RUBBER SITUATION '' ( PDF ). International Rubber Study Group. Nov 2014. Archived from the original ( PDF ) on 12 April 2015. Retrieved 2015 - 12 - 27. Jump up ^ Dr. Aye Aye Khin. `` The Impact of the Changes of the World Crude Oil Prices on the Natural Rubber Industry in Malaysia ''. Jump up ^ Listiyorini, Eko ( 2010 - 12 - 16 ). `` Rubber Exports From Indonesia May Grow 6 % - 8 % Next Year ''. bloomberg.com. Archived from the original on 4 November 2012. Retrieved 2013 - 03 - 21. Jump up ^ This section has been copied almost verbatim from the public domain UN Food and Agriculture Organization ( FAO ), ecoport.com article : Cecil, John ; Mitchell, Peter ; Diemer, Per ; Griffee, Peter ( 2013 ). `` Processing of Natural Rubber, Manufacture of Latex - Grade Crepe Rubber ''. ecoport.org. FAO, Agricultural and Food Engineering Technologies Service. Retrieved March 19, 2013. Jump up ^ Basic Rubber Testing. ASTM International. pp. 6 --. GGKEY : 8BT2U3TQN7G. Jump up ^ Transportation of Natural Rubber - Industry Source Jump up ^ Horath, Larry ( 2017 - 03 - 17 ). Fundamentals of Materials Science for Technologists : Properties, Testing, and Laboratory Exercises, Second Edition. Waveland Press. ISBN 9781478635185. Jump up ^ `` Rubber Faqs ''. ^ Jump up to : `` Premarket Notification ( 510 ( k ) ) Submissions for Testing for Skin Sensitization To Chemicals In Natural Rubber Products '' ( PDF ). FDA. Retrieved 22 September 2013. Jump up ^ `` New Type of Latex Glove Cleared ''. Jump up ^ American Latex Allergy Association. `` Allergy Fact Sheet ''. Jump up ^ Rook, J.J. ( 1955 ). `` Microbiological deterioration of vulcanized rubber ''. Appl. Microbiol. 3 : 302 -- 309. Jump up ^ Leeang, K.W.H. ( 1963 ). `` Microbiologic degradation of rubber ''. J. Am. Water Works Assoc. 53 : 1523 -- 1535. Jump up ^ Tsuchii, A. ; Suzuki, T. ; Takeda, K. ( 1985 ). `` Microbial degradation of natural rubber vulcanizates ''. Appl. Environ. Microbiol. 50 : 965 -- 970. Jump up ^ Heisey, R.M. ; Papadatos, S. ( 1995 ). `` Isolation of microorganisms able to metabolize puri ¢ ed natural rubber ''. Appl. Environ. Microbiol. 61 : 3092 -- 3097. Jump up ^ Jendrossek, D. ; Tomasi, G. ; Kroppenstedt, R.M. ( 1997 ). `` Bacterial degradation of natural rubber : a privilege of actinomycetes ? ''. FEMS Microbiology Letters. 150 : 179 -- 188. doi : 10.1016 / s0378 - 1097 ( 97 ) 00072 - 4. Jump up ^ Linos, A. and Steinbuchel, A. ( 1998 ) Microbial degradation of natural and synthetic rubbers by novel bacteria belonging to the genus Gordona. Kautsch. Gummi Kunstst. 51, 496 - 499. Jump up ^ Linos, Alexandros ; Steinbuchel, Alexander ; Spröer, Cathrin ; Kroppenstedt, Reiner M. ( 1999 ). `` Gordonia polyisoprenivorans sp. nov., a rubber degrading actinomycete isolated from automobile tire ''. Int. J. Syst. Bacteriol. 49 : 1785 -- 1791. PMID 10555361. doi : 10.1099 / 00207713 - 49 - 4 - 1785. Jump up ^ Linos, Alexandros ; Reichelt, Rudolf ; Keller, Ulrike ; Steinbuchel, Alexander ( October 1999 ). `` A Gram - negative bacterium, identified as Pseudomonas aeruginosa AL98, is a potent degrader of natural rubber and synthetic cis - 1, 4 - polyisoprene ''. FEMS Microbiology Letters. 182 : 155 -- 161. doi : 10.1111 / j. 1574 - 6968.2000. tb08890. x. Jump up ^ Helge B. Bode ; Axel Zeeck ; Kirsten Plückhahn ; Dieter Jendrossek ( September 2000 ). `` Physiological and Chemical Investigations into Microbial Degradation of Synthetic Poly ( cis - 1, 4 - isoprene ) ''. Applied and Environmental Microbiology. 66 ( 9 ) : 3680 -- 3685. PMC 92206. PMID 10966376. doi : 10.1128 / AEM. 66.9. 3680 - 3685.2000. Bibliography Ascherson, Neal ( 1999 ). The King Incorporated : Leopold the Second and the Congo. Granta Books. ISBN 978 - 1 - 86207 - 290 - 9. ( 1999 Granta edition ). Brydson, J.A. ( 30 November 1988 ). Rubbery Materials and their Compounds. Springer Netherlands. ISBN 978 - 1 - 85166 - 215 - 9. Hobhouse, Henry ( 2005 ) ( 2003 ). Seeds of Wealth : Five Plants That Made Men Rich. Shoemaker & Hoard. pp. 125 -- 185. ISBN 1 - 59376 - 089 - 2. Hochschild, Adam ( 2002 ). King Leopold 's Ghost : A Story of Greed, Terror, and Heroism in Colonial Africa. Pan. ISBN 978 - 0 - 330 - 49233 - 1. Morton, M. ( 17 April 2013 ). Rubber Technology. Springer Science & Business Media. ISBN 978 - 94 - 017 - 2925 - 3. Petringa, Maria ( 13 January 2006 ). Brazzà, A Life for Africa. AuthorHouse. ISBN 978 - 1 - 4520 - 7605 - 8. External links Look up natural rubber in Wiktionary, the free dictionary. Media related to Rubber at Wikimedia Commons Non-timber forest products Animal products Furs Honey Pine honey Wild game Berries Tree fruit Blackberry Blueberry Bilberry Breadfruit Cocoa bean Coconut Durian Gambooge Huckleberry Jackfruit Juniper berry Lingonberry Raspberry Tamarind Woodland strawberry Edible plants / roots Betel Fiddlehead ferns Mahuwa flowers Sago palm queen Sassafras filé powder root beer Saw palmetto Wild ginseng Mushrooms Bare - toothed russula Bay bolete Birch bolete Cep Chanterelle Honey mushroom Lingzhi Matsutake Meadow mushroom Morel Oyster mushroom Parasol mushroom Red cap Saffron milk cap Slippery jack Truffle Yellow knight Nuts Spices Allspice Areca nut Bay leaf Black pepper Brazil nut Cinnamon Clove Hazelnut Malva nut Nutmeg Pine nut Vanilla Oil Waxes Carnauba Chaulmoogra ( Hydnocarpus wightiana ) Cocoa butter Eucalyptol Eucalyptus Japan wax Kokum Kusum Mahuwa Nagkesar Palm ( kernel ) Pongamia Phulwara Pilu Sal - seed ( Shorea robusta ) Sandalwood Shea butter Tea - seed Tea - tree Vateria indica Resins Benzoin Birch tar Camphor Creosote Frankincense Gamboge Kauri Lacquer Mastic Myrrh Pine tar Pitch Rosin Turpentine Varnish Sap / Gum / etc. Birch syrup Chicle chewing gum Coconut sugar Date sugar Fruit syrup Gum arabic Gutta - percha Kino Latex Maple sugar Maple syrup Palm sugar Palm wine akpeteshie ogogoro Rubber Spruce gum Other Bamboo edible musical instruments textiles Birch bark Birch beer Cork Ferns Forage Gambier Moss Natural dyes henna Peat Quinine Rattan Shellac Tanbark tannin Thatching Tendu leaves Willow bark Related Dehesa ( Iberian agroforestry ) Forest farming / gardening Honey hunting Indian forest produce Mushroom hunting Naval stores Permaforestry Resin extraction Rubber tapping Wildcrafting Forestry portal Trees portal Commons WikiProject Forestry Types of Terpenes and Terpenoids ( # of isoprene units ) Basic forms : Acyclic ( linear, cis and trans forms ) Monocyclic ( single ring ) Bicyclic ( 2 rings ) Iridoids ( cyclopentane ring ) Iridoid glycosides ( iridoids bound to a sugar ) Steroids ( 4 rings ) Hemiterpenoids ( 1 ) Isoprene ( C H ) Prenol Isovaleric acid Monoterpene ( C H ) ( 2 ) Acyclic Ocimene Myrcenes Monocyclic Limonene Terpinene Phellandrene Umbellulone Bicyclic Pinene ( β and α Camphene Thujene Sabinene Carene Monoterpenoids ( 2, modified ) Acyclic Linalool Citronellal Citral Citronellol Geraniol Geranyl pyrophosphate Monocyclic Grapefruit mercaptan menthol p - Cymene thymol Perillyl alcohol Carvacrol Bicyclic Camphor Borneol Eucalyptol Halomon Eucalyptol Pinene Ascaridole Sesquiterpenoids ( 3 ) Farnesyl pyrophosphate Artemisinin Bisabolol Diterpenoids ( 4 ) Geranylgeranyl pyrophosphate Gibberellin Retinol Retinal Phytol Taxol Forskolin Aphidicolin Salvinorin A Sesterterpenoids ( 5 ) geranylfarnesol Triterpenoids ( 6 ) Steroids Phytosterols Campesterol beta Sitosterol gamma sitosterol Stigmasterol Tocopherols Cholesterol Testosterone Cholecalciferol ( Vit D ) Ecdysones Other Saponins Squalane Lanosterol Acids Oleanolic acid Ursolic acid Betulinic acid Moronic acid Sesquarterpenes / oids ( 7 ) ferrugicadiol tetraprenylcurcumene Tetraterpenoids ( Carotenoids ) ( 8 ) Carotenes Alpha - Carotene Beta - Carotene Gamma - Carotene Delta - Carotene Lycopene Neurosporene Phytofluene Phytoene Xanthophylls : Canthaxanthin Cryptoxanthin Zeaxanthin Astaxanthin Lutein Rubixanthin Polyterpenoids ( many ) sap, resins, latex of many plants, e.g. rubber Norisoprenoids ( modified ) 3 - oxo - α - ionol 7, 8 - dihydroionone Synthesis Terpene synthase enzymes ( many ), having in common a Terpene synthase N terminal domain ( protein domain ) Activated isoprene forms Isopentenyl pyrophosphate ( IPP ) Dimethylallyl pyrophosphate ( DMAPP ) GND : 4022538 - 0 NDL : 00562543 Retrieved from `` https://en.wikipedia.org/w/index.php?title=Natural_rubber&oldid=804268977 '' Categories : Natural materials Organic polymers Terpenes and terpenoids Rubber Adhesives Nonwoven fabrics Forestry in Thailand Forestry in Indonesia Forestry in Malaysia History of forestry Non-timber forest products Crops Thermoplastic elastomers Hidden categories : Articles needing additional references from September 2016 All articles needing additional references Use dmy dates from January 2013 Articles needing additional references from August 2015 Articles needing additional references from November 2016 Articles that may contain original research from November 2016 All articles that may contain original research All articles with specifically marked weasel - worded phrases Articles with specifically marked weasel - worded phrases from February 2017 Wikipedia articles with GND identifiers Talk Contents About Wikipedia Afrikaans Azərbaycanca Беларуская Bosanski Català Čeština Cymraeg Deutsch Eesti Ελληνικά Español Esperanto Euskara فارسی Français Frysk Gaeilge Galego 贛 語 ગુજરાતી 한국어 Հայերեն हिन्दी Hrvatski Ido Bahasa Indonesia Íslenska Italiano עברית ಕನ್ನಡ ქართული Қазақша Kongo Latina Latviešu Lietuvių Limburgs Magyar മലയാളം Bahasa Melayu Mirandés မြန်မာဘာသာ Nāhuatl Nederlands 日本 語 Norsk Norsk nynorsk Occitan Patois Polski Português Română Русский Sicilianu සිංහල Simple English Slovenščina Српски / srpski Srpskohrvatski / српскохрватски Basa Sunda Suomi Svenska தமிழ் Татарча / tatarça తెలుగు ไทย Türkçe Тыва дыл Українська اردو Vèneto Tiếng Việt West - Vlams Winaray ייִדיש 粵語 中文 Edit links This page was last edited on 7 October 2017, at 21 : 42. Text is available under the Creative Commons Attribution - ShareAlike License ; additional terms may apply. By using this site, you agree to the Terms of Use and Privacy Policy. Wikipedia ® is a registered trademark of the Wikimedia Foundation, Inc., a non-profit organization. About Wikipedia

Question: where does most of the world's rubber come from
Answer: Thailand